annotation to the lesson 5 elastomeric impression materials elastomeric impression materials ... the
Post on 21-Mar-2020
Embed Size (px)
ANNOTATION TO THE LESSON № 5
ELASTOMERIC IMPRESSION MATERIALS
The impression materials discussed so far are not good enough generally for taking accurate impressions of the dental patient. The alginates arc inherently weak materials and provide poor reproduction of surface detail; agar is dimensionally unstable and only suitable if laboratory facilities arc close at hand; and the rigid impression materials cannot be removed from deep undercuts. Thus, there is still a need for an impression material that is accurate, that shows a large recoverable deformation, and has adequate long-term (dimensional stability. These goals can all be met with the elastomeric impression materials.
The elastomeric impression materials arc characterised as polymers that are used at a temperature above their glass transition temperature. Such materials become more and more fluid as their temperature is raised above their glass transition temperature, Tg.
The viscosities of the polymers that are used for impression materials are governed primarily by the molecular weight of the polymer (i.e. the length of the polymer chains) and by the presence of additives, such as fillers. Thus, we have a material that is fluid at room temperature, but that can be turned into a solid by binding the long-chain molecules together. This process of binding the chains to form a three-dimensional network is known as cross-linking and forms the basis of the liquid-to-solid transition or all the elastomeric impression materials. There are essentially three main groups of elastomeric impression materials:
ü polysulphides ü polyethers ü silicones (C-type and A-type). Each group the elastomers is classified according to its viscosity. In the table
№1 4 viscosity types of the elastomeric impression materials are presented.
Types of the elastomers (ISO4823:1992) Type (ISO)
Characteristic of viscosity ( a disc diameter in mm)
0 1 2 3
(P) putty (H) high
(M) middle (L) low
≤ 30 20 - 31 31 - 36 36 min
Polysulfide rubber (mercaptan)
Polysulfide rubbers are widely used for fixed partial denture application, due to their high accuracy and relatively low cost. These materials are useful for multiple impressions when extra time is needed. The polysulfides are supplied in tubes of base paste and catalyst paste, which are mixed together. Polysulfides are available in low, medium, and high viscosities.
Composition The base paste contains the polysulfide polymer, fillers, and plasticizers. The content of the reinforcing fillers (eg, zinc oxide, titanium dioxide, zinc sulfide, and silica) varies from 12% to 50% depending on the consistency (light, regular, or heavy). The fillers and plasticizers control the stiffness of the paste. The accelerator or catalyst paste contains lead dioxide (30%), hydrated copper oxide or organic peroxide, as a catalyst; sulfur (1% to 4%) as a promoter; and dibutyl phthalate or other nonreactive oils (17%) to form a paste. The balance of the catalyst paste is inorganic fillers used to adjust the consistency and reactivity. Those materials containing an organic peroxide may have decreased dimensional stability due to evaporation of the peroxide. Note that this is a condensation polymerization with water as a by-product. Mechanical properties
For elastic recovery, the polysulfides have values of about 96%, slightly lower than those for the other rubber impression materials (eg, silicone and polyether). Values for flow range from 0.4% to 1.9%, indicating a tendency to distort upon storage. The flow tends to be highest for the light-bodied and least for the heavy bodied materials. Light-bodied polysulfides have flexibilities of about 16%; regular bodied polysulfides have values of about 14%; and heavy- bodied polysulfides have values of about 10%. This is an advantage over the stiffer addition silicones and polyethers because removal from undercut areas is
easier. Polysulfides have the highest tear strength of the rubber materials, which allows their use in deep subgingival areas where removal is difficult. Manipulation
These materials are mixed on a mixing pad with a spatula. Equal lengths of base and catalyst are extruded on a disposable mixing pad. The components are mixed thoroughly with a stiff tapered spatula. The catalyst is dark and the base is white so thorough mixing is readily observed by lack of streaks in the mix. Adequate mixing time is 45 to 60 seconds. The working time is about 5 to 7 minutes , which is adequate considering the mixing times. Both working and setting times are shortened by higher temperatures and humidity. A value of 0.45% is given for shrinkage after 24 hours. Although this is less than that of the condensation silicones, the cast or die should be poured within 1 hour of taking the impression. Since polysulfides take longer to set than silicones, they require more chair time. They stain clothing permanently. They can be electroplated; some products can be silverplated, but copperplating is not recommended.
Advantages Advantages of polysulfides include a long working time, good tear strength, good flow before setting, good reproduction of surface detail, high flexibility for easier removal around undercuts, and lower cost compared to silicones and polyethers.
Disadvantages Disadvantages of these materials include the need to use custom-made rather than stock trays due to a greater chance of distortion, a bad odor, a tendency to run down the patient's throat due to lower viscosity, and the lead dioxide materials that stain clothing. Polysulfides must be poured within 1 hour and cannot be repoured.
Troubleshooting Sometimes problems may be encountered when using polysulfide rubber impression materials: 1. Inadequate working time. This could result from excessive humidity and/or temperature. An increase in either of these variables results in decreased working and setting times. An improper base-to-catalyst ratio could also produce inadequate working time (too much catalyst will reduce working time).
2. Distortion. A number of factors cause distortion, one of which is too much load. Because recovery after deformation is dependent on the amount and duration of loading, the impression should not be placed face down on the laboratory bench.
Improper removal from the mouth could also cause distortion of the impression; removal should be rapid because permanent deformation is a function of duration of stress. If a bubble is located just below the surface adjacent to a preparation (internal porosity), the impression may distort.
3. Loss of detail. Premature removal from the mouth may be a cause of this. Removal prior to sufficient polymerization or before the material is sufficiently elastic will result in inaccurate registration of detail. This may also be the result of incomplete mixing; failure to incorporate all the catalyst into the base will result in incomplete polymerization of portions of the surface. Movement of the tray prior to the time of removal could also cause loss of detail. The impression tray should be held firmly until the elastic stage is attained.
4. Surface bubbles or voids. These could be caused by the incorporation of air into the mix. The impression material should always be mixed carefully with only the flat surface of the blade. If the material is partially polymerized prior to insertion in the mouth, voids may occur in the impression.
Disinfection Polysulfide impressions can be disinfected by immersion in sodium
hypochlorite, iodophors, complex phenolics, glutaraldehydes, or phenolic glutaraldehydes. The manufacturer's recommendations for proper disinfection should be followed.
Silicone rubber condensation type Condensation silicone rubber impression materials are used mainly for
fixed partial denture impressions. They are ideal for single-unit inlays. These materials are supplied either as two-paste or paste-liquid catalyst systems. Condensation silicones are available in low, medium, high, and very high (putty) viscosities.
Composition The base paste usually contains a moderately high-molecular-weight
poly(dimethylsiloxane) with terminal hydroxy groups (-OH), an orthoalkylsilicate for cross-linking, and inorganic filler. A paste will contain 30% to 40% filler, whereas a putty will contain as much as 75%. The catalyst paste or liquid usually contains a metal organic ester, such as tin octoate or dibutyl tin dilaurate, and an oily diluent. A thickening agent is used when making catalyst
pastes. Sometimes a catalyst will contain both the orthoalkylsilicate and the metal organic ester. A volatile alcohol is formed as a by-product.
Mechanical properties Accepted values for the mechanical properties of these materials are given
in An average value of 99% for elastic recovery is excellent. The flow of silicones is low; most values are less than 0.1%, indicating that less distortion is likely to be caused by light pressure on standing. The silicones are stiffer than polysulfides, as indicated by lower flexibility values in The shrinkage in 24 hours ranges from 0.2% to 1.0%. About half the shrinkage takes place in the first hour, and it is greater than for polysulfides or polyethers. Polymerization and evaporation of the alcohol formed in the reaction are responsible for this high shrinkage. Accuracy is greatly improved by first taking an impression with a highly filled silicone putty and, after setting, t